Synthesis of Microfiber with Secondary Nanostructure by Cotton Template
Hierarchical microfibers were prepared by using cotton as the template and as the precursor via an ultrasonic assistance route. The results of scanning electron microscope characterization showed that the concentration of had a significant effect on the morphology of microfiber. At low concentration of , the microfiber was composed of nanorods with single crystal structure. With increasing the concentration of , the secondary nanostructure of microfibers had a transformation from nanorod to nanoparticle. The results of adsorption-desorption analysis indicated that microfibers had BET surface area of about 25 /g. This synthesis provides a new way to control the secondary nanostructure of microfiber by adjusting the concentration of precursor. Furthermore, the mechanism for the replication was proposed and discussed.
In recent years, many templates, such as mesoporous silica [1, 2], AAO [3–5], and surfactant micelle [6, 7], have been used for the preparation of nanostructured oxides. Biological materials have also been used as templates or scaffolds for the preparation of nanostructured oxides because of their interesting structures [8, 9]. In comparison with other templates, biological materials are “green” and easy to obtain. In the process of replication, the structure of biological materials provides a stable and controllable condition to guide the assembly of nanostructured oxides. The obtained nanostructured oxides can replicate the characteristic structures or even the functionalities of biological materials [10, 11]. Different species of biological materials, such as wood [12–14], filter paper [15, 16], and sisal , were used for the fabrication of various inorganic nanomaterials. In comparison with other kinds of plant fibers, the morphology of cotton fiber is more uniform.
In the past few years, MnO2 nanomaterials have attracted considerable attention due to their potential applications in the areas of catalyst, ion-sieves, and electrode materials . Recently, Zhu et al. prepared a series of manganese oxides via a “green” biotemplating method . Herein, we fabricated microfibers with secondary nanostructure by using cotton as the template and KMnO4 as the precursor. The effect of the concentration of KMnO4 on the morphology of MnO2 microfibers was studied and the possible formation mechanism was also discussed.
2. Experimental Section
Medical absorbent cotton was used as the template. It was pretreated before use. The cotton was immersed in 5 wt% HCl aqueous solution for 3 hours, washed with distilled water, and dried at 80°C in air. Then the sample was immersed in 6 wt% NaOH aqueous solution for 3 hours at 60°C, washed with distilled water, and dried at 80°C in air.
1.0 g of the pretreated cotton was dispersed in KMnO4 aqueous solution in a beaker. The beaker was exposed to ultrasonic irradiation (100 W) for 6 hours. The sample was taken out, washed ten times with distilled water, and dried at 80°C in air. Then the sample was calcined at 500°C for 3 hours in air. Finally, the sample was washed with distilled water and alcohol to remove the byproduct, and then dried at 80°C in air. The concentrations of KMnO4 aqueous solution were 5, 10, and 20 g/mL, respectively. The as-prepared samples were denoted as sample 1, sample 2, and sample 3, respectively. Furthermore, the sample without calcination process was denoted as the precursor/cotton.
The crystal structure of the sample was characterized by X-ray diffraction (XRD) (Bruker D8 advance). The morphology of the sample was examined by scanning electron microscopy (SEM Gemini LEO1530) and transmission electron microscopy (TEM JEOL JEM-2100). The N2 adsorption-desorption analysis was measured on a Micromeritics ASAP 2010 instrument.
3. Results and Discussion
The XRD pattern of the precursor/cotton of sample 1 is shown in Figure 1a. Two peaks can be seen at about 15° and 23°. It is difficult to judge the phase of the sample. Then the precursor/cotton was calcined to remove the cotton template. XRD patterns of sample 1 and sample 3 are shown in Figures 1(b), and 1(c), respectively. The results indicate that the samples are MnO2 with a tetragonal structure (JCPDS 44-0141).
Figures 2(a) and 2(b) show the SEM images of the precursor/cotton of sample 1. Figures 2(c) and 2(d) shows the SEM images of the sample 1. Compared with the precursor/cotton sample, the obtained MnO2 sample replicates the fiber structure of the cotton, but with some shrinkage in size. Figures 2(b) and 2(d) indicated that the surface morphology of MnO2 microfiber is obviously different from the precursor/cotton sample. MnO2 microfiber is composed of abundant nanorods. The TEM image (Figure 2(f)) also indicates that the microfiber is composed of nanorods. The corresponding selected-area electron diffraction (SAED) pattern (the inset in Figure 2(f)) indicates that the nanorods possess single crystal structure. The HRTEM images of the nanorods are shown in Figures 2(g) and 2(h). A layer separation of about 0.69 nm can be observed, which is corresponding to the value of the (110) planes of MnO2.
Figure 3 shows the SEM images of sample 2 and sample 3. From the pictures, it can be seen that sample 2 is composed of nanoparticles and nanorods. Sample 3 is composed of nanoparticles. Therefore, it can be concluded that the secondary structure of the microfibers has a transformation from nanorod to nanoparticle with increasing the concentration of KMnO4. In addition, the nanostructure of the microfibers becomes dense with increasing the concentration of KMnO4.
The N2 adsorption-desorption isotherms and the corresponding BJH pore-size distributions of MnO2 microfibers are shown in Figure 4. All the samples have a sorption isotherm with a clear capillary condensation step in a relative pressure range of 0.9–1.0 (Figure 4(a)), implying the porous structure with large pore size. The porous structure was mainly produced from the stack of the nanomaterials. The BJH pore-size distributions indicate that all the samples possess large pore-size and broad pore distributions. The Brunauer-Emmett-Teller (BET) surface areas for sample 1, sample 2, and sample 3 are 24.8, 26.1, and 23.6 m2/g, respectively. The pore volumes for sample 1, sample 2, and sample 3 are 0.12, 0.14, and 0.14 cm3/g, respectively.
The formation mechanism of the samples is studied. The purpose of the pretreatment for the cotton is to remove the lignin and form R-CH2ONa, which make access the hierarchical pore channels more easily because of the resulting high porosity and the ionic environment . The hydroxyl groups of the cotton facilitate the complexation of ions with the cotton. In order to investigate the effect of ultrasonic irradiation, comparative experiment was performed. It is found that the precursor adsorbed on the cotton is very little if without the ultrasonic irradiation. The high-intensity ultrasound through water can lead to acoustic cavitation, which is the formation, growth, and violent collapse of gas microbubbles in the solution. The near adiabatic compression of the gas molecules inside the microbubbles in the liquid leads to a dramatic rise in the temperature and pressure within the bubbles , and this can have the effect of generating reactive free-radical species ( ions) in solution. The flow of solution made from the gas microbubbles leads to more into the channels of cotton. The cotton fiber not only serves as the template for the formation of microfiber, but also provides the location for the nucleation and the growth of MnO2 nanostructure during the heat treatment. Moreover, the hydroxyl groups of the cotton act as passivation contacts for the stabilization of the nanoparticles formed inside the cotton. In addition, the concentration of the precursor plays an important role in the morphology of MnO2 nanostructure. The SEM results (Figures 2(e) and 3(b)) indicated that the nanostructure becomes dense with increasing the concentration of KMnO4. Thus, we think that the growth void of crystals determines the final morphology of the nanostructure. The nanorod structure can be obtained only when the growth void is enough.
In conclusion, hierarchical MnO2 microfibers with secondary nanostructure were successfully prepared by using cotton as the template and as the precursor via an ultrasound route. The microfibers with secondary nanostructure may be found to potential applications in the areas of catalyst, ion-sieve, and electrode material. It is expected that this biotemplating method can be extended to other metal oxide materials.
This work was supported by Natural Science Foundation of Jiangsu Province (BK2006195).
M.-B. Zheng, J. Cao, S.-T. Liao et al., “Preparation of mesoporous nanoparticles via solid-liquid route and effects of calcination temperature and textural parameters on their electrochemical capacitive behaviors,” Journal of Physical Chemistry C, vol. 113, no. 9, pp. 3887–3894, 2009.View at: Publisher Site | Google Scholar
P. Yang, D. Zhao, D. I. Margolese, B. F. Chmelka, and G. D. Stucky, “Block copolymer templating syntheses of mesoporous metal oxides with large ordering lengths and semicrystalline framework,” Chemistry of Materials, vol. 11, no. 10, pp. 2813–2826, 1999.View at: Google Scholar
G. Ji, Z. Gong, W. Zhu et al., “Simply synthesis of nanowire arrays using a solvent-free method,” Journal of Alloys and Compounds, vol. 476, no. 1-2, pp. 579–583, 2009.View at: Publisher Site | Google Scholar
W.-S. Chae, S.-W. Lee, and Y.-R. Kim, “Templating route to mesoporous nanocrystalline titania nanofibers,” Chemistry of Materials, vol. 17, no. 12, pp. 3072–3074, 2005.View at: Publisher Site | Google Scholar
X. Wang, X. Wang, W. Huang, P. J. Sebastian, and S. Gamboa, “Sol-gel template synthesis of highly ordered nanowire arrays,” Journal of Power Sources, vol. 140, no. 1, pp. 211–215, 2005.View at: Publisher Site | Google Scholar
G. Liu, B. Xie, D. Fu, Y. Wang, Q. Fu, and D. Wang, “Preparation of nearly monodisperse microcapsules with controlled morphology by in situ polymerization of a shell layer,” Journal of Materials Chemistry, vol. 19, no. 36, pp. 6605–6609, 2009.View at: Publisher Site | Google Scholar
Q. Zhou, X. Li, Y.-G. Li, B.-Z. Tian, D.-Y. Zhao, and Z.-Y. Jiang, “Synthesis and electrochemical properties of semicrystalline gyroidal mesoporous ,” Chinese Journal of Chemistry, vol. 24, no. 7, pp. 835–839, 2006.View at: Publisher Site | Google Scholar
S. Sotiropoulou, Y. Sierra-Sastre, S. S. Mark, and C. A. Batt, “Biotemplated nanostructured materials,” Chemistry of Materials, vol. 20, no. 3, pp. 821–834, 2008.View at: Publisher Site | Google Scholar
N. Ma, E. H. Sargent, and S. O. Kelley, “Biotemplated nanostructures: directed assembly of electronic and optical materials using nanoscale complementarity,” Journal of Materials Chemistry, vol. 18, no. 9, pp. 954–964, 2008.View at: Publisher Site | Google Scholar
D. Zhang and L. Qi, “Synthesis of mesoporous titania networks consisting of anatase nanowires by templating of bacterial cellulose membranes,” Chemical Communications, no. 21, pp. 2735–2737, 2005.View at: Publisher Site | Google Scholar
W. Zhang, D. Zhang, T. Fan et al., “Novel photoanode structure templated from butterfly wing scales,” Chemistry of Materials, vol. 21, no. 1, pp. 33–40, 2009.View at: Publisher Site | Google Scholar
T. Fan, X. Li, J. Ding, D. Zhang, and Q. Guo, “Synthesis of biomorphic based on natural plant templates and assembly of Ag nanoparticles controlled within the nanopores,” Microporous and Mesoporous Materials, vol. 108, no. 1–3, pp. 204–212, 2008.View at: Publisher Site | Google Scholar
A. Dong, Y. Wang, Y. Tang et al., “Zeolitic tissue through wood cell templating,” Advanced Materials, vol. 14, no. 12, pp. 926–929, 2002.View at: Publisher Site | Google Scholar
T. Ota, M. Imaeda, H. Takase et al., “Porous titania ceramic prepared by mimicking silicified wood,” Journal of the American Ceramic Society, vol. 83, no. 6, pp. 1521–1523, 2000.View at: Google Scholar
J. Huang, I. Ichinose, and T. Kunitake, “Biomolecular modification of hierarchical cellulose fibers through titania nanocoating,” Angewandte Chemie International Edition, vol. 45, no. 18, pp. 2883–2886, 2006.View at: Publisher Site | Google Scholar
J. Huang, N. Matsunaga, K. Shimanoe, N. Yamazoe, and T. Kunitake, “Nanotubular templated by cellulose fibers: synthesis and gas sensing,” Chemistry of Materials, vol. 17, no. 13, pp. 3513–3518, 2005.View at: Publisher Site | Google Scholar
J. He and T. Kunitake, “Preparation and thermal stability of gold nanoparticles in silk-templated porous filaments of titania and zirconia,” Chemistry of Materials, vol. 16, no. 13, pp. 2656–2661, 2004.View at: Publisher Site | Google Scholar
H. Zhang, G. Cao, Z. Wang, Y. Yang, Z. Shi, and Z. Gu, “Growth of manganese oxide nanoflowers on vertically-aligned carbon nanotube arrays for high-rate electrochemical capacitive energy storage,” Nano Letters, vol. 8, no. 9, pp. 2664–2668, 2008.View at: Publisher Site | Google Scholar
S. Zhu, D. Zhang, Z. Li, H. Furukawa, and Z. Chen, “Precision replication of hierarchical biological structures by metal oxides using a sonochemical method,” Langmuir, vol. 24, no. 12, pp. 6292–6299, 2008.View at: Publisher Site | Google Scholar
Y. Cao, J. Cao, J. Liu, M. Zheng, and K. Shen, “Sonochemical fabrication and photoluminescence properties of ordered mesopogpus carbon-tin oxide nanocomposites,” Chemistry Letters, vol. 36, no. 2, pp. 254–255, 2007.View at: Publisher Site | Google Scholar